In strained mechanical resonators, the concurrence of tensile stress and geometric nonlinearity dramatically reduces dissipation. This phenomenon, called dissipation dilution, is employed in mirror suspensions of gravitational-wave interferometers and at the nanoscale, where soft clamping and strain engineering have allowed extremely high quality factors. However, these techniques have so far been applied only to amorphous materials, specifically Si3N4. Crystalline materials exhibit substantially lower intrinsic damping at cryogenic temperatures. Applying dissipation dilution engineering to strained crystalline materials could, therefore, enable extremely low loss nanomechanical resonators, as they combine low internal friction, high intrinsic strain and high yield strength. This potential has not yet been fully exploited. Here we demonstrate that single-crystal strained silicon—a material developed for high-mobility transistors—can be used to realize mechanical resonators with ultralow dissipation. We fabricate strained silicon nanostrings with high aspect ratios supporting megahertz mechanical modes with quality factors exceeding 1010 at 7 K, a tenfold improvement over values reported in Si3N4. We estimate a thermal-noise-limited force sensitivity of (5 ± 2) × 10–20 N Hz–1/2 at 7 K—approaching that of carbon nanotubes—and a heating rate of only 60 quanta per second. The low mass and high quality factors of our nanomechanical resonators make them particularly promising for quantum sensing and transduction.
This is a preview of subscription content, access via your institution
Open Access articles citing this article.
Hierarchical tensile structures with ultralow mechanical dissipation
Nature Communications Open Access 02 June 2022
Access Nature and 54 other Nature Portfolio journals
Get Nature+, our best-value online-access subscription
$29.99 per month
cancel any time
Subscribe to this journal
Receive 12 print issues and online access
$209.00 per year
only $17.42 per issue
Rent or buy this article
Get just this article for as long as you need it
Prices may be subject to local taxes which are calculated during checkout
Source data are provided with this paper. Data supporting the figures and lithographic masks used for microfabrication are available on Zenodo (https://doi.org/10.5281/zenodo.4606602).
Braginskiĭ, V. B., Mitrofanov, V. P. & Panov, V. I. Systems with Small Dissipation (Univ. Chicago Press, 1985).
Cady, W. G. The piezo-electric resonator. Proc. Inst. Radio Eng. 10, 83–114 (1922).
Braginsky, V. B., Gorodetsky, M. L. & Vyatchanin, S. P. Thermodynamical fluctuations and photo-thermal shot noise in gravitational wave antennae. Phys. Lett. A 264, 1–10 (1999).
Hirose, E. et al. Sapphire mirror for the KAGRA gravitational wave detector. Phys. Rev. D 89, 062003 (2014).
Cole, G. D., Zhang, W., Martin, M. J., Ye, J. & Aspelmeyer, M. Tenfold reduction of Brownian noise in high-reflectivity optical coatings. Nat. Photon. 7, 644–650 (2013).
Kessler, T. et al. A sub-40-mHz-linewidth laser based on a silicon single-crystal optical cavity. Nat. Photon. 6, 687–692 (2012).
Chae, J., Kulah, H. & Najafi, K. A monolithic three-axis micro-g micromachined silicon capacitive accelerometer. J. Microelectromech. Syst. 14, 235–242 (2005).
Rugar, D., Budakian, R., Mamin, H. J. & Chui, B. W. Single spin detection by magnetic resonance force microscopy. Nature 430, 329–332 (2004).
Degen, C. L., Poggio, M., Mamin, H. J., Rettner, C. T. & Rugar, D. Nanoscale magnetic resonance imaging. Proc. Natl Acad. Sci. USA 106, 1313–1317 (2009).
Safavi-Naeini, A. H. et al. Squeezed light from a silicon micromechanical resonator. Nature 500, 185–189 (2013).
Cripe, J. et al. Measurement of quantum back action in the audio band at room temperature. Nature 568, 364–367 (2019).
Phillips, W. A. Two-level states in glasses. Rep. Prog. Phys. 50, 1657–1708 (1987).
Pohl, R. O., Liu, X. & Thompson, E. Low-temperature thermal conductivity and acoustic attenuation in amorphous solids. Rev. Mod. Phys. 74, 991–1013 (2002).
Grabovskij, G. J., Peichl, T., Lisenfeld, J., Weiss, G. & Ustinov, A. V. Strain tuning of individual atomic tunneling systems detected by a superconducting qubit. Science 338, 232–234 (2012).
Bagdasarov, S., Braginsky, V. B. & Mitrofanov, V. P. Mechanical dissipation in single crystal sapphire. Kristallografiya 19, 883 (1974).
Galliou, S. et al. Extremely low loss phonon-trapping cryogenic acoustic cavities for future physical experiments. Sci. Rep. 3, 2132 (2013).
McGuigan, D. F. et al. Measurements of the mechanical Q of single-crystal silicon at low temperatures. J. Low Temp. Phys. 30, 621–629 (1978).
Unterreithmeier, Q. P., Faust, T. & Kotthaus, J. P. Damping of nanomechanical resonators. Phys. Rev. Lett. 105, 027205 (2010).
Yu, P.-L., Purdy, T. P. & Regal, C. A. Control of material damping in high-Q membrane microresonators. Phys. Rev. Lett. 108, 083603 (2012).
Fedorov, S. A. et al. Generalized dissipation dilution in strained mechanical resonators. Phys. Rev. B 99, 054107 (2019).
Nowick, A. S. Anelastic Relaxation In Crystalline Solids (Academic Press, 1972).
Tsaturyan, Y., Barg, A., Polzik, E. S. & Schliesser, A. Ultracoherent nanomechanical resonators via soft clamping and dissipation dilution. Nat. Nanotechnol. 12, 776–783 (2017).
Reetz, C. et al. Analysis of membrane phononic crystals with wide band gaps and low-mass defects. Phys. Rev. Appl. 12, 044027 (2019).
Bereyhi, M. J. et al. Clamp-tapering increases the quality factor of stressed nanobeams. Nano Lett. 19, 2329–2333 (2019).
Beccari, A. et al. Hierarchical tensile structures with ultralow mechanical dissipation. Preprint at https://arxiv.org/abs/2103.09785 (2021).
Ghadimi, A. H. et al. Elastic strain engineering for ultralow mechanical dissipation. Science 360, 764–768 (2018).
Bereyhi, M. J. et al. Nanomechanical resonators with ultra-high-Q perimeter modes. Preprint at https://arxiv.org/abs/2108.03615 (2021).
Villanueva, L. G. & Schmid, S. Evidence of surface loss as ubiquitous limiting damping mechanism in SiN micro- and nanomechanical resonators. Phys. Rev. Lett. 113, 227201 (2014).
Rossi, M., Mason, D., Chen, J., Tsaturyan, Y. & Schliesser, A. Measurement-based quantum control of mechanical motion. Nature 563, 53–58 (2018).
Tao, Y. et al. Permanent reduction of dissipation in nanomechanical Si resonators by chemical surface protection. Nanotechnology 26, 465501 (2015).
Liu, J. et al. High-Q optomechanical GaAs nanomembranes. Appl. Phys. Lett. 99, 243102 (2011).
Romero, E. et al. Engineering the dissipation of crystalline micromechanical resonators. Phys. Rev. Appl. 13, 044007 (2020).
Kermany, A. R. et al. Microresonators with Q-factors over a million from highly stressed epitaxial silicon carbide on silicon. Appl. Phys. Lett. 104, 081901 (2014).
Cole, G. D. et al. Tensile-strained InxGa1–xP membranes for cavity optomechanics. Appl. Phys. Lett. 104, 201908 (2014).
Bückle, M. et al. Stress control of tensile-strained In1–xGaxP nanomechanical string resonators. Appl. Phys. Lett. 113, 201903 (2018).
Chu, M., Sun, Y., Aghoram, U. & Thompson, S. E. Strain: a solution for higher carrier mobility in nanoscale MOSFETs. Annu. Rev. Mater. Res. 39, 203–229 (2009).
Jacobsen, R. S. et al. Strained silicon as a new electro-optic material. Nature 441, 199–202 (2006).
MacCabe, G. S. et al. Nano-acoustic resonator with ultralong phonon lifetime. Science 370, 840–843 (2020).
Ghyselen, B. et al. Engineering strained silicon on insulator wafers with the Smart CutTM technology. Solid State Electron. 48, 1285–1296 (2004).
Hÿtch, M., Houdellier, F., Hüe, F. & Snoeck, E. Nanoscale holographic interferometry for strain measurements in electronic devices. Nature 453, 1086–1089 (2008).
De Wolf, I., Maes, H. E. & Jones, S. K. Stress measurements in silicon devices through Raman spectroscopy: bridging the gap between theory and experiment. J. Appl. Phys. 79, 7148–7156 (1996).
Süess, M. J. et al. Power-dependent Raman analysis of highly strained Si nanobridges. Nano Lett. 14, 1249–1254 (2014).
Schmid, S., Jensen, K. D., Nielsen, K. H. and Boisen, A. Damping mechanisms in high-Q micro and nanomechanical string resonators. Phys. Rev. B 84, 165307 (2011).
Honig, R. E. & Hook, H. O. Vapor pressure data for some common gases. RCA Rev. 21, 360–368 (1960).
Cannelli, G. et al. Reorientation of the B-H complex in silicon by anelastic relaxation experiments. Phys. Rev. B 44, 11486–11489 (1991).
Gysin, U. et al. Temperature dependence of the force sensitivity of silicon cantilevers. Phys. Rev. B 69, 045403 (2004).
Sementilli, L., Romero, E. & Bowen, W. P. Nanomechanical dissipation and strain engineering. Adv. Funct. Mater. 32, 2105247 (2022).
Carney, D. et al. Mechanical quantum sensing in the search for dark matter. Quantum Sci. Technol. 6, 024002 (2021).
Boureau, V., Reboh, S., Benoit, D., Hÿtch, M. & Claverie, A. Strain evolution of SiGe-on-insulator obtained by the Ge-condensation technique. APL Mater. 7, 041120 (2019).
Hopcroft, M. A., Nix, W. D. & Kenny, T. W. What is the Young’s modulus of silicon? J. Microelectromech. Syst. 19, 229–238 (2010).
Flinn, P. A., Gardner, D. S. & Nix, W. D. Measurement and interpretation of stress in aluminum-based metallization as a function of thermal history. IEEE Trans. Electron Devices 34, 689–699 (1987).
Chen, W. W., Sun, X. H., Wang, S. D., Lee, S. T. & Teo, B. K. Etching behavior of silicon nanowires with HF and NH4F and surface characterization by attenuated total reflection Fourier transform infrared spectroscopy: similarities and differences between one-dimensional and two-dimensional silicon surfaces. J. Phys. Chem. B 109, 10871–10879 (2005).
Norte, R. A. Nanofabrication for On-Chip Optical Levitation, Atom-Trapping, and Superconducting Quantum Circuits. PhD thesis, California Institute of Technology (2015).
Borselli, M., Johnson, T. J. & Painter, O. Measuring the role of surface chemistry in silicon microphotonics. Appl. Phys. Lett. 88, 131114 (2006).
Anastassakis, E., Pinczuk, A., Burstein, E., Pollak, F. H. & Cardona, M. Effect of static uniaxial stress on the Raman spectrum of silicon. Solid State Commun. 8, 133–138 (1970).
Ossikovski, R., Nguyen, Q., Picardi, G., Schreiber, J. & Morin, P. Theory and experiment of large numerical aperture objective Raman microscopy: application to the stress-tensor determination in strained cubic materials. J. Raman Spectrosc. 39, 661–672 (2008).
Hart, T. R., Aggarwal, R. L. & Lax, B. Temperature dependence of Raman scattering in silicon. Phys. Rev. B 1, 638–642 (1970).
Anastassakis, E., Cantarero, A. & Cardona, M. Piezo-Raman measurements and anharmonic parameters in silicon and diamond. Phys. Rev. B 41, 7529–7535 (1990).
Catalini, L., Tsaturyan, Y. & Schliesser, A. Soft-clamped phononic dimers for mechanical sensing and transduction. Phys. Rev. Appl. 14, 014041 (2020).
We thank D. Wilson and A. Ghadimi for their contributions in the early stages of the project, and R. Groth for assistance with sample characterization. This work was supported by funding from the Swiss National Science Foundation under grant agreement no. 182103, the EU H2020 research and innovation programme under grant agreement no. 732894 (HOT) and the European Research Council grant no. 835329 (ExCOM-cCEO). N.J.E. acknowledges support from the Swiss National Science Foundation under grant no. 185870 (Ambizione). This work was further supported by the Defense Advanced Research Projects Agency (DARPA), Defense Sciences Office (DSO) contract no. HR00111810003. All the samples were fabricated at the Center of MicroNanoTechnology (CMi) at EPFL.
The authors declare no competing interests.
Peer review information
Nature Physics thanks Christopher Baker and the other, anonymous, reviewer(s) for their contribution to the peer review of this work.
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Extended Data Fig. 1 Fabrication of sSi nanostrings.
a, Suspended nanostrings without a stress-compensation layer are subject to a compressive load well beyond the critical value for out-of-plane buckling. Green - SiO2, blue - patterned sSi + FOX16 mask. b, The encapsulation layers (dark and light green) compensate compressive stress; the suspended beam is tensioned and flat. c, Determination of the intrinsic stress in PECVD SixNy through wafer bow. The wafer height profile is measured by scanning a laser beam and recording the angular deflection of the beam reflected off the surface. The magnitude and sign of the profile curvature permit to reconstruct the biaxial stress. Red circles - wafer profile before nitride deposition, orange circles - wafer bow after nitride deposition, with the initial profile subtracted.
Extended Data Fig. 2 Color-coded strain map in sSi, measured with dark-field electron holography.
a, Portion of Fig. 2f magnified around the sSi layer. b, Distribution of reconstructed strain values in the sSi layer, centered on the average strain 〈ϵ〉 = 0.85%.
Extended Data Fig. 3 Raman scans with variable laser power.
Micro-Raman scans along a PnC beam unit cell are conducted, with variable laser power. A linear dependence of the Raman scattering wavevector on the power is observed; the dotted line indicates the extrapolation to zero optical power.
Extended Data Fig. 4 Schematic of the measurement setup.
ECDL: external cavity diode laser. EOM: electro-optical modulator. WDM: fiber optic wavelength division multiplexer. PZT: piezoelectric transducer. ESA: spectrum analyzer.
Extended Data Fig. 5 Comparison of ringdowns with continuous and gated acquisition.
The probe laser, with an impinging power ≿ 1 mW, induces, in the continuous ringdown (green line), additional optical damping, leading to a faster amplitude decay rate than the one set by the intrinsic dissipation of the nanostring. For the gated ringdown (blue dots), the measurement duty cycle (ratio of gate duration over the time interval between successive gates) is 10%, and the gate repetition rate is 1/20 s. In both ringdowns, nonlinear damping is observed at the highest amplitudes59, and exponential fits (dashed lines) are performed only within the linear decay regions. The data were acquired at T ≈ 10 K for the 6.0 mm sample presented in the main text.
Source Data Fig. 3
Plain text data for Fig. 3.
Source Data Fig. 4
Plain text data for Fig. 4.
Rights and permissions
About this article
Cite this article
Beccari, A., Visani, D.A., Fedorov, S.A. et al. Strained crystalline nanomechanical resonators with quality factors above 10 billion. Nat. Phys. 18, 436–441 (2022). https://doi.org/10.1038/s41567-021-01498-4
This article is cited by
Hierarchical tensile structures with ultralow mechanical dissipation
Nature Communications (2022)
Good vibrations for quantum computing
Nature Physics (2022)